Arch Toxicol DOI 10.1007/s00204-014-1245-3
The optical, photothermal, and facile surface chemical properties of gold and silver nanoparticles in biodiagnostics, therapy, and drug delivery Lauren A. Austin · Megan A. Mackey · Erik C. Dreaden · Mostafa A. El‑Sayed
Received: 7 April 2014 / Accepted: 15 April 2014 © Springer-Verlag Berlin Heidelberg 2014
Abstract Nanotechnology is a rapidly growing area of research in part due to its integration into many biomedical applications. Within nanotechnology, gold and silver nanostructures are some of the most heavily utilized nanomaterial due to their unique optical, photothermal, and facile surface chemical properties. In this review, common colloid synthesis methods and biofunctionalization strategies of gold and silver nanostructures are highlighted. Their unique properties are also discussed in terms of their use in biodiagnostic, imaging, therapeutic, and drug delivery applications. Furthermore, relevant clinical applications utilizing gold and silver nanostructures are also presented. We also provide a table with reviews covering related topics. Keywords Silver nanostructures · Gold nanostructures · Localized surface plasmon resonance (LSPR) · Surface-enhanced Raman scattering (SERS) · Plasmonic photothermal therapy (PPTT) · Biofunctionalization
Introduction The rapid development of nanotechnology has had an invaluable impact on the biomedical field. Nanoparticles, i.e., materials with overall dimensions between 1 and 100 nm,
L. A. Austin · M. A. Mackey · M. A. El‑Sayed (*) Laser Dynamics Laboratory, Department of Chemistry and Biochemistry, Georgia Institute of Technology, 901 Atlantic Dr. NW, Atlanta, GA 30332‑0400, USA e-mail: [email protected]
E. C. Dreaden Koch Institute for Integrative Cancer Research, Department of Chemical Engineering, Massachusetts Institute of Technology, 500 Main St., Cambridge, MA 02139, USA
have been utilized in many biomedical applications as contrast agents and biosensors and in therapeutic delivery (Caro et al. 2010; Dreaden et al. 2012a; Murthy 2007). Their nanometer size makes them biologically relevant as they have the ability to permeate cellular membranes and interact with important biomolecules, such as DNA, proteins, and viruses. Additionally, they exhibit several unique properties that differ greatly from their bulk counterparts. Noble metal nanostructures, such as gold and silver, have attracted much attention due to their unique photothermal, chemical, and optical properties (Table 1) (Jain et al. 2007, 2008). Owing to their nanometer size, they exhibit large surface-to-volume ratios that can be leveraged in therapeutic delivery applications. The surface of gold (AuNPs) and silver (AgNPs) nanostructures is also chemical reactive allowing for facile functionalization with various biological stabilizing agents, biomolecules, and chemotherapeutic agents. Their most distinguishable physical property is their enhanced optical performance (i.e., light scattering and absorption). Their remarkable optical properties originate from their unique interaction with light resulting in the collective coherent oscillation of their free conduction band electrons, or the localized surface plasmon resonance (LSPR). The oscillation of the free electrons decays via two processes: (1) radiative decay resulting in the very strong visible scattering of light and (2) nonradiative decay resulting in the conversion of photon energy into thermal energy (Jain et al. 2008). These two decay mechanisms have been readily utilized in biodiagnostic and imaging (exploiting radiative SPR decay), and therapeutic (exploiting nonradiative SPR decay) applications. In this review, we will discuss common Au and Ag nanostructure syntheses and biofunctionalization approaches as well as some of their biodiagnostic, therapeutic, and clinical applications.
Table 1 A compilation of reviews related to Au and Ag nanostructures for biomedical applications Application
Antimicrobial Wound Healing Antiviral
Grzelczak et al. (2008), Lu et al. (2009b), Quang Huy et al. (2013), Tao et al. (2008), Yu et al. (2008) Ju et al. (2011), Mout et al. (2012), Sapsford et al. (2013), Sperling and Parak (2010) Petryayeva and Krull (2011), Willets and Van Duyne (2007) Jain et al. (2007), Li et al. (2012), Murphy et al. (2008) Jain et al. (2008), Kneipp et al. (2010), Qian and Nie (2008), Schlücker (2009), Tripp et al. (2008), Vo-Dinh et al. (2010) Aslan et al. (2005), Lakowicz (2006) Chen et al. (2013), Höppener and Novotny (2012) Dreaden et al. (2011), Huang et al. (2008), Jain et al. (2008) Dreaden et al. (2011), Ghosh et al. (2008), Kumar et al. (2013), Pissuwan et al. (2011), Vigderman and Zubarev (2013) Boisselier and Astruc (2009), Dreaden et al. (2011), Ghosh et al. (2008), Jeong et al. (2014), Pissuwan et al. (2011), Vigderman and Zubarev (2013) Rai et al. (2009), Sharma et al. (2009), Vigderman and Zubarev (2013) Tocco et al. (2012) Arvizo et al. (2012), Galdiero et al. (2011), Sharma et al. (2009)
Arvizo et al. (2012), Boisselier and Astruc (2009), Dreaden et al. (2011)
Biofunctionalization Localized surface plasmon resonance (LSPR) shift Enhanced rayleigh scattering Surface-enhanced Raman scattering (SERS) Metal-enhanced fluorescence Nanoparticle surface energy transfer (NSET) Plasmonic photothermal therapy (PPTT) Drug Delivery Gene therapy
It should be noted that this is not a comprehensive list
Synthesis Gold and silver nanostructures synthesized for biological applications are commonly prepared using the colloidal synthesis method. This approach utilizes a metal precursor, a reducing agent, and a stabilizing agent, and allows for the facile tuning of the size, shape, and optical properties of the nanostructures. Some of the syntheses for gold and silver nanostructures are highlighted below. Gold nanostructures Gold nanospheres (AuNSs) One of the most widely used gold nanostructures is spherical gold nanoparticles (AuNSs) as they can be easily synthesized in large quantities with relatively high monodispersity (Fig. 1a). Spherical gold nanoparticles, which were first reported by Faraday in 1857, are generally synthesized using Turkevich’s citrate reduction method (Faraday 1857; Turkevich et al. 1951). This method produces spherical particles with diameters ≥10 nm and involves the reduction of aqueous chloroauric acid by sodium citrate. By varying the stoichiometric ratio between gold and the reducing agent, sodium citrate, the size of the spherical nanoparticles can be controlled, with larger ratios leading to particles with larger diameters (Frens 1973). In this method, citrate not only acts as the reducing agent, but it also stabilizes the particles via electrostatic repulsion. In the event that spherical gold nanoparticles of diameters ≤10 nm are required, the Brust method is generally employed (Brust
et al. 1994). Developed in 1994, this method involves a two-phase system where gold ions are reduced by sodium borohydride (NaBH4) at an oil–water interface, and tetraoctylammonium bromide (TOAB) is used as the phase transfer catalyst and stabilizing agent. Due to the relatively weak binding between TOAB and the spherical gold nanoparticles, alkanethiols are introduced to prevent aggregation. Most recently, in 2009, Perrault and Chen developed a method complementary to the citrate reduction method to produce highly monodispersed spherical gold nanoparticles with diameters of 50–200 nm (Perrault and Chan 2009). In this synthesis, hydroquinone is used to reduce chloroauric acid onto the surface of gold nanoparticle seeds. The addition of sodium citrate was shown to improve particle stability and monodispersity at large diameters. Gold nanorods (AuNRs) Gold nanorods (AuNRs) are another commonly synthesized gold nanostructure as they are readily used in photothermal and NIR applications (Fig. 1b). There are two general colloidal approaches to gold nanorod synthesis: seed-mediated and seedless growth. The seed-mediated growth method was first described by Murphy et al. in 2001 and further explored by Nikoobakt and ElSayed in 2003 (Jana et al. 2001a; Nikoobakht and El-Sayed 2003). This method, often referred to as the seed-mediated growth method, requires a solution of small seeds (3–5 nm) produced from the reduction of chloroauric acid by NaBH4 in the presence of CTAB. Once formed, the seeds are introduced into a gold (I) growth solution containing ascorbic
Fig. 1 Commonly synthesized Au and Ag nanostructures for biodiagnostic and therapeutic applications. Graphical illustrations, electron micrographs, and extinction spectra for a Au nanospheres, b Au nanorods, c Au nanocages, d Ag nanospheres, e Ag nanorods, and f Ag nanocubes. Observed red-shift in extinction spectra is representative of increasing nanostructure size (a, d, f), increasing aspect ratio (b, e), and increasing gold deposition (c). Reprinted with permission from a (Link and El-Sayed 1999), b (Huang et al. 2009), c (Skra-
balak et al. 2008) and (Chen et al. 2006), d (Pyatenko et al. 2007), e (Mahmoud and El-Sayed 2013), and f (Mahmoud and El-Sayed 2012) and (Chen et al. 2006). Copyright. 1999 American Chemical Society, 2009 Wiley–VCH Verlag GmbH & Co. KGaA, 2008 American Chemical Society, 2006 American Chemical Society, 2007 American Chemical Society, 2013 American Chemical Society, 2012 American Chemical Society, and 2006 American Chemical Society, respectively
acid, silver nitrate (AgNO3), and CTAB. The seeds serve as nucleation sites for Au+ anisotropic reduction to form gold nanorods with transverse diameters similar to those synthesized by the electrochemical method. While the transverse diameter is relatively constant at 10 nm, the length and in turn the aspect ratio of the nanorod can be adjusted by increasing the concentration of AgNO3. Recently, both Murphy and El-Sayed groups have investigated the synthesis of smaller gold nanorods from the seedless growth method (Ali et al. 2012; Jana et al. 2001b). In this synthesis, the growth solution is kept at an acidic pH via the addition of hydrochloric acid, and NaBH4 is added to simultaneously initiate seed formation and gold nanorod growth. The resulting gold nanorods have dimensions of 28 × 8 nm.
replacement spontaneously occurs because the reduction potential of silver is less than gold, which leads to the oxidization and displacement of silver atoms as gold atoms are reduced onto the nanocube surface. The cage-like structure is formed from voids due to gold reduction occurring in a threeelectron process, while the oxidation of silver occurs in a oneelectron process (i.e., three silver atoms are replaced by one gold atom). The synthesized gold nanocages have a typical edge length of 40 nm and a wall thickness of 3.5 nm.
Gold nanocages (AuNCs) As recently as 2005, Xia and coworkers have developed another gold nanostructure that has impacted the field of biomedicine (Chen et al. 2005). Gold nanocages (AuNCs), which have exploitable optical properties along with a hollow interior structure, are synthesized via the galvanic replacement method (Fig. 1c) (Chen et al. 2006; Skrabalak et al. 2008). This method uses silver nanocubes, previously synthesized by the polyol reduction of AgNO3, as the sacrificial template for gold nucleation and growth. The
Silver nanostructures Silver nanospheres (AgNSs) Spherical silver nanoparticles (AgNSs) are one of the most commonly synthesized silver nanostructures (Fig. 1d). Although spherical silver nanoparticles can be synthesized using the Turkevich method that was previously described for spherical gold nanoparticles, this method tends to produce large particle diameters (50– 100 nm) with broad surface plasmon absorption when using citrate as the reducing and capping agent (Turkevich et al. 1951). In order to obtain smaller spherical nanoparticles (5–20 nm), NaBH4 usually replaces citrate as the reducing agent (Fang 1998). More recently, Suzuki and coworkers described a combined seed and laser technique to produce
spherical silver nanospheres with diameters ranging from 10–80 nm (Pyatenko et al. 2007). Silver colloid seeds with an average diameter of 8–10 nm were produced via citrate reduction of silver nitrate and subsequent irradiation by the second harmonic Nd/YAG laser (λ = 532 nm). The silver seeds were then subjected to either a one-step or multistep synthesis, which involves the addition of the silver seeds to a boiling solution of citrate and AgNO3, to produce larger spherical particles with relatively high monodispersity. Silver nanocubes (AgNCs) Another frequently utilized silver nanostructure in the biomedical field is the silver nanocube (AgNC) as they exhibit enhanced scattering that can be exploited in biological sensing applications (Fig. 1e). First introduced by Xia and coworkers in 2002, silver nanocubes are synthesized by the polyol method, which involves the reduction of AgNO3 with ethylene glycol and utilizes poly(vinyl pyrrolidone) (PVP) as the capping agent (Sun and Xia 2002). This method is kinetically controlled as maintaining a relatively high final silver nitrate concentration and a relatively low molar ratio between PVP and silver nitrate. This allows for the fast nucleation and growth of silver seeds in addition to preventing the formation of twin defects. The fast nucleation and growth reduce twin defect formation. By varying the silver nitrate concentration and growth time, the size of the nanocubes can be controlled.
stability. This affords facile surface functionalization with various biological and organic molecules. The relative ease of nanoparticle surface modification, through noncovalent and covalent interactions, allows for not only the replacement of potentially toxic initial stabilizing agents, such as CTAB, but also allows for specific biological targeting, and their use in biodiagnostic and biosensing applications. Noncovalent modifications occur through electrostatic interactions, hydrophobic entrapment, and van der Walls forces, while covalent modifications utilize direct chemical attachment, linker molecules, or click chemistry. Noncovalent interactions
Silver nanorods (AgNRs) Silver nanorods (AgNRs) are another silver nanostructure that are heavily utilized due to their enhanced biosensing ability (Fig. 1f). Jana et al. (2001c) described a silver nanorod synthesis that is similar to that reported for gold nanorods and produces silver nanorods with lengths that are much small than that achieved by the electrochemical method. In this synthesis, silver seeds with a diameter of 4 nm are produced from the NaBH4 reduction of AgNO3 in an aqueous citrate solution. Once the seeds are prepared, AgNO3 is reduced by ascorbic acid in a solution containing the silver seeds, the cationic surfactant CTAB, and sodium hydroxide (NaOH). Larger aspect ratios are achieved through decreasing the amount of silver seeds present in the nanorod growth solution. When using 4 nm silver seeds, silver nanorods with a length of ~42 nm and an aspect ratio of 3.5 are produced. More recently, Mahmoud et al. (2013) were able to synthesize AgNRs with different aspect ratios by using the polyol reduction method at high temperatures and high stirring speeds. The high temperatures and stirring speeds aided in overcoming the thin layer formed around the nanorod surface that is believed to stop nanorod growth.
Electrostatic interactions have been extensively used to functionalize gold and silver nanoparticles to biomolecules, such as DNA, peptides, and antibodies. This mode of functionalization relies on the attraction between two oppositely charged species: the nanoparticle surface and the biomolecule of interest (Fig. 2). The advantage of this interaction is that the biomolecule is not exposed to harsh chemical modifications that could compromise its native, active form. When using this type of nanoparticle functionalization, it is important to consider the impact of the surrounding medium’s ionic strength and pH. In 2001, Rotello and coworkers utilized this interaction to functionalize cationic gold clusters with DNA using the negatively charged phosphate backbone of DNA (McIntosh et al. 2001). The stability of the DNA-functionalized gold clusters was confirmed via UV–Vis spectroscopy and dynamic light scattering (DLS). Our group has also used electrostatic interactions to functionalize AuNPs and AuNRs with anti-EGFR antibodies to selectively target and photothermally destroy cancer cells (Huang et al. 2006a, b, 2007). Electrostatic interactions were also used by Yuan et al. (2012) to immobilize an antineurogenin 1 (anti-ngn 1) antibody on dl-mercaptosuccinic acid (MSA) stabilized AgNPs. The interaction was established between the anionic carboxyl groups (–COO−) of the MSA-AgNPs and the cationic amine groups (–NH3+) of the antibody and enabled the label-free detection of the synthetic peptide fragment of ngn 1. Rotello and coworkers further exploited noncovalent interactions to successfully load hydrophobic therapeutics, tamoxifen, and βlapachone, to AuNPs (Kim et al. 2009). The AuNPs were designed such that they mimicked micelle structures (i.e., a hydrophobic interior and a hydrophilic exterior), which allowed for the encapsulation of hydrophobic drugs in the hydrophobic pockets.
One of the most advantageous properties of gold and silver nanostructures in the biomedical field is their surface
While noncovalent attachment to the nanoparticle surface has its advantages, covalent interactions generally provide
Arch Toxicol Fig. 2 Common functionalization strategies for Au and Ag nanostructures for use in biomedical applications
greater stability and reproducibility of molecular functionalization (Fig. 2). Chemisorption, or dative bonding, is commonly used to attach thiol-terminated biomolecules and biopolymers to nanoparticle surfaces through strong metal-S bonds. For example, the bond energy between Au and S is 44 kcal mol−1 (Dubois and Nuzzo 1992). This interaction is achieved when the sulfur atom donates a lone pair of electrons to the empty orbitals of gold or silver atoms at an interface (Sapsford et al. 2013). Thiolated biopolymers such as PEG and polyoxazoline (POx) have been anchored to gold nanoparticle surfaces through Au–S bonds to enhance the particle’s stability in physiological environments as well as avoid nonspecific binding of serum proteins and opsonization when introduced into in vivo systems (Amoozgar and Yeo 2012; Wang et al. 2011b). Other biocompatible polymers used for physiological nanoparticle stabilization are PVP, poly(styrene sulfonate) (PSS), and poly(lysine) (PLL). Metal-S bond formation has also been used to adhere oligonucleotides to nanoparticle surfaces. Both Mirkin and Alivisatos independently demonstrated oligonucleotide-functionalized AuNPs in 1996, and this work has since been extended to various biomedical applications such as hepatitis C virus detection, intracellular gene regulation, and mercuric ion detection (Alivisatos et al. 1996; Glynou et al. 2003; Lee et al. 2007; Mirkin et al. 1996; Rosi et al. 2006). Targeting ligands such as arginine–glycine–aspartic acid (RGD) and nuclear localizing signal (NLS) peptides have also been conjugated to gold and silver nanoparticle surfaces
through the metal-S bond to promote particle internalization by human oral squamous cell (HSC-3) cells and their subsequent nuclear localization (Austin et al. 2011a; Kang et al. 2010a; Oyelere et al. 2007). Functionalization in this system occurred via cysteine residues located within the peptides and the nanoparticle surface. Many nanoparticle conjugate systems utilize bifunctionalized linkers to covalently attach therapeutic drugs and biomolecules as this reduces the possibility of undesirable structural changes that may arise from direct interaction. It has been demonstrated that proteins that directly interact with the nanoparticle surface, such as those seen in the protein corona, may undergo conformational changes that alter their biological activity (Lundqvist et al. 2008). Commonly used linkers for biomedical applications include oligoethylene glycol (OEG) and PEG polymers modified with amine (–NH3+), carboxyl (–COO−), isothiocyanate (–N=C=S), or maleimide (H2C2(CO)2NH) functional groups. These functional groups allow for conventional coupling strategies, such as carbodiimide-mediated esterification and amidation (Fig. 2) (Liu et al. 2010b). The linker molecules are also modified to contain thiol or disulfide groups to promote their exchange with capping agents at the nanoparticle surface. Prabaharan et al. (2009) demonstrated the successful covalent attachment of doxorubicin (DOX) to a hydrophobic inner layer of a folic acid amphiphilic AuNP via a pH-sensitive hydrazone linkage. Their folate-targeted DOX-conjugated AuNP showed selective uptake and DOX release to breast cancer cells. Ying and coworkers also
used covalently attached DOX to AgNPs to create a DNA biosensor (Ting et al. 2009). DOX was bound to aminefunctionalized AgNPs using an NHS-PEG-NHS linker. Moreover, tumor-targeting antibodies, such as single-chain variable fragment (ScFv) antibodies, have been conjugated to nanoparticles using heterobifunctional PEG linkers and EDC/NHS coupling (Qian et al. 2008). Click chemistry, most notably azide-alkyne Huisgen cycloaddition, which involves the use of a copper catalyst, has also been utilized for nanoparticle functionalization and related applications (Fischler et al. 2008; Zhu et al. 2012). Imaging and biodiagnostic applications As stated previously, noble metal nanostructures offer unique physical and optical properties that can be exploited in in vitro and in vivo imaging and diagnostic applications. Their nanometer size is comparable to many important biological molecules (i.e., DNA, proteins, viruses, etc.) and allows them to penetrate cellular and tumorigenic systems. Even more beneficial than size are their optical properties, namely their ability to strongly scatter light and enhance the local electric field (Jain et al. 2007, 2008). These properties, stemming from surface plasmon resonance, are readily utilized to lower biomarker detection limits, monitor disease progression, and identify diseased systems. LSPR shift One of the most unique properties of Au and Ag nanostructures is LSPR. LSPR is the coherent oscillation of the nanostructure’s conduction band free electrons in resonance with the incident electromagnetic field. A metallic nanostructure’s LSPR is highly dependent on the size, shape, and dielectric constant of the nanostructure as well as the dielectric function of the surrounding medium (Jain et al. 2007, 2008). Due to the sensitivity of a nanostructure’s LSPR to its surrounding environment, biosensors based on the shift of the LSPR have been developed (Petryayeva and Krull 2011). There are two general approaches to LSPR sensors: (1) shifts due to nanostructure aggregation and (2) shifts resulting from biomolecule–surface interactions. The first approach is based on the interparticle plasmon coupling between nanostructures as the interparticle distance changes. Since a nanostructure’s electromagnetic field (EM) is localized at the surface and decays exponentially as the distance away from the surface is increased, interparticle coupling is maximized when nanostructures are in an aggregated state (Jain et al. 2006; Petryayeva and Krull 2011). The aggregated state results in a red-shift of the LSPR and is often noticeable to the naked eye via color change of the nanostructure in solution (e.g., gold nanosphere aggregation is indicated by a color change from red
Fig. 3 Colorimetric detection of mercuric ion using DNA-AuNPs. a Schematic diagram of the colorimetric Hg2+ assay. AuNPs were divided into two groups and functionalized with complementary DNA that contains a thymidine–thymidine mismatch as indicated in red. In the presence of Hg2+, the DNA-AuNPs will form aggregates due to Hg2+ coordination at the T–T mismatch site. b The presence and concentration of Hg2+ ions can be determined by the color change (or LSPR shift) of the solution at a given temperatures. Reprinted with permission from (Lee et al. 2007). Copyright. 2007 Wiley–VCH Verlag GmbH & Co. KGaA
to blue). The relationship between the LSPR shift and the interparticle distance is shown in Eq. 1 (Willets and Van Duyne 2007): −2d LSPR, max = mn 1 − exp (1) Id where m is the bulk refractive index of the nanostructure [in nm per refractive index unit (RIU)], Δn is the change in the refractive index (in RIU), d is the effective thickness of the absorbant layer (in nm), and Id is the characteristic EM field decay length (in nm). One of the first reports of using aggregation-based LSPR sensing came from Mirkin et al. (1996) (Elghanian et al. 1997). In this study, two sets of 13 nm AuNPs were functionalized with noncomplementary strands of oligonucleotides via thiol groups. When the two noncomplementary oligonucleotide-AuNPs were introduced into a solution containing complementary ssDNA, the solution’s color changed from red to blue indicating the successful hybridization between the ssDNA target and the oligonucleotideAuNPs. Mirkin and coworkers have further expanded this ssDNA oligonucleotide-AuNP sensor to single-nucleotide
base detection and metal ion detection (Fig. 3) (Lee et al. 2007; Storhoff et al. 1998). Aslan et al. (2004) employed aggregation-based LSPR sensing in the detection of glucose using dextran-coated nanogold. In this work, dextran-AuNPs were initially aggregated using concanavalin A (Con A), a carbohydrate-binding protein. The addition of glucose, which competitively binds to Con A, reduced nanogold aggregation, resulting in a LSPR blue shift as well as a decrease in the plasmon absorbance at the aggregated wavelength (650 nm). Moreover, silver nanoparticle LSPR aggregation assays have been utilized to detect enzyme reactions, such as those involving the consumption of adenosine triphosphate (ATP) (Wei et al. 2008). The second approach to LSPR shift assays originates from the sensitivity of the LSPR to the refractive index near the nanostructure surface as demonstrated in Eq. 1. As the equation parameters indicate, the use of this assay is for situations in which the absorbant layer is negligible and the analyte of interest is located within the near field of the nanostructure surface (Petryayeva and Krull 2011). To assess assay performance, a sensitivity factor (SF) was used. The SF is defined as the LSPR wavelength shift per unit change in the effective refractive index of the surrounding medium and is expressed in units of nm RUI−1. Our group as well as others has shown that a nanoparticle’s SF, due to its dependence on the LSPR, is greatly affected by the shape, size, and metal choice (Haes et al. 2004b; Lee and El-Sayed 2006; Liu and Huang 2013; Sherry et al. 2005). An early investigation, conducted by Englebienne, showed the use of the LSPR shift to infer apparent affinity constants between protein antigens and antibodies (Englebienne 1998). The LSPR shift was detected using an automated photometer and produced results that were in good agreement with those determined from traditional methods (i.e., Scatchard plots). Nath et al. later applied this approach in a planar, chip-based format in an attempt to detect biotin–streptavidin binding using a UV-visible spectrophotometer (Nath and Chilkoti 2001). AuNPs that were immobilized on a transparent substrate to allow for UVvisible spectroscopic measurements were functionalized with biotin and incubated with increasing concentrations (e.g., 0.3–100 μg/mL) of streptavidin. A detection limit of ~1 μg/mL and a dynamic range of ~1–30 μg/mL were achieved, which demonstrated the analytical sensitivity of this assay. Since these initial “proof of concept” experiments, the LSPR shift principle has been applied to Alzheimer’s disease detection (Ag nanotriangles), the simultaneous detection of pathogenic Escherichia coli (E. coli) and Salmonella tryphimurium (AuNRs with varying aspect ratios), neurotransmitter detection (multiblock Au and Ag NRs, AuNPs), and glucose detection (AgNSs) (Baron et al. 2005; Choi et al. 2013; Haes et al. 2004a; Tashkhourian et al. 2011; Wang and Irudayaraj 2008).
Enhanced Rayleigh scattering Au and Ag nanostructures exhibit enhanced Rayleigh (elastic) scattering originating from their LSPR. The resulting scattered light is heavily dependent on the nanostructure shape and size, as larger nanostructures and those that contain corners (i.e., cubes, cages, etc.) scatter light more strongly (Jain et al. 2007, 2008). Their enhanced light scattering provides several advantages when used as a biological imaging or sensing agent. The scattered light is much brighter (4–5 orders of magnitude) than the most efficient fluorophores, is much stronger than background sample matrices, is resistant to photobleaching, and does not require expensive strong excitation sources. Enhanced Rayleigh scattering has been readily used for cellular imaging and utilizes a conventional light microscope equipped with a dark field condenser. The dark field condenser is used to allow only the sample’s scattered light, which is at the frequency of the SPR, to be collected by the microscope’s objective. In 2005, El-Sayed et al. (2005) demonstrated the great sensitivity of using dark field light scattering to identify cancerous cells. AuNPs were labeled with anti-epidermal growth factor receptor (anti-EGFR) antibodies, which specifically target the EGFR protein on cell membranes. Cancerous cells are known to have significantly higher EGFR protein expression on their cell membrane when compared to healthy cells. Anti-EFGR conjugated AuNPs were incubated with cancerous and healthy cells and imaged using a dark field microscopy. It was evident from dark field images that the cancerous cells exhibited stronger light scattering resulting from the specific labeling of the anti-EFGF-AuNPs. El-Sayed and coworkers have also used the enhanced light scattering in a dark field arrangement to identify AuNP and AgNP nuclear localization after conjugation with nuclear localizing sequence (NLS) peptides (Fig. 4a) (Austin et al. 2011a; Kang et al. 2010a; Mackey et al. 2013; Oyelere et al. 2007). Austin et al. (2011b) utilized AgNP light scattering to image cancer cell communities during programmed cell death. Human oral squamous cell carcinoma (HSC-3) cells were incubated with increasing concentrations of nucleartargeted AgNPs, which were previously shown to induce apoptosis. Dark field microscopy was used to image the treated cell communities for ~24 h and captured nonprofessional phagocytic activity and cellular clustering as a result of nuclear-targeted AgNP incubation. Recently, antibodyfunctionalized AuNPs that are specific for E. coli were used as light scattering reporters to quantify bacteria colonies (Xu et al. 2012). This method provided a detection limit of ~104 CFU/mL and was obtained within 15–30 min. In addition to cellular imaging, the plasmonically enhanced light scattering can also be used in biomarker or analyte detection. As mentioned previously, the LSPR is
Fig. 4 Surface-enhanced Rayleigh scattering applications of AuNPs. a Dark field light scattering was utilized to assess AuNR (left) and peptide-conjugated AuNR (right) uptake. Peptide conjugation determined to promote AuNR cellular uptake. Scale bar 10 μM. (b) Schematic diagram of fPSA detection using antibody-conjugated AuNSs and AuNRs (left). Nanoparticle incubation with fPSA caused two hydrodynamic diameter populations correlating to oligomer formation (right A and inset) and individual particles (right B). The peak area ratio between population A and population B reveals fPSA concentrations. a Reprinted with permission from (Oyelere et al. 2007). Copyright. 2007 American Chemical Society. b Reprinted with permission from (Liu et al. 2008). Copyright. 2008 American Chemical Society
strongly affected by changes in the refractive index of the surrounding medium and thus can shift upon changes in molecule–surface interactions. The LSPR is composed of both absorption and scattering components, and therefore, a shift in the LSPR results in a shift of the light scattering wavelength. Since LSPR shift assays were discussed in detail in the above section, other light scattering sensors will be highlighted. Du et al. (2008) utilized the enhanced light scattering of antibody-AuNPs to develop a homogeneous noncompetitive immunoassay that was consistent with traditional enzyme-linked immunosorbent assays (ELISA). The concentration-dependent increase in AuNP light scattering, after the addition of a model analyte, provided a detection limit of 10 ng/mL and allowed for analyte detection in human serum samples. Moreover, dynamic light scattering (DLS) has been coupled with Au nanoprobes to detect important biomolecules, such as free prostatespecific antigen (f-PSA) and target DNA sequences (Dai et al. 2008; Jans et al. 2009; Liu et al. 2008). In the former, Huo and coworkers conjugated capture and detector anti-PSA antibodies to AuNSs and AuNRs, and quantified the amount f-PSA present through the formation of dimers, trimers, and oligomers (Fig. 4b) (Liu et al. 2008). DLS-AuNP coupled biomolecule detection provides many advantages, such as simple sample preparation, a one-step homogenous assay format, and orders of magnitude in sensitivity enhancement.
Surface‑enhanced Raman scattering (SERS) Raman spectroscopy is a spectroscopic technique that provides details about the vibrational modes in a system. This technique is based on the inelastic scattering of photons, usually from monochromatic (i.e., laser) light. The energy difference (i.e., frequency shift) between the incident light and the Raman scattered light is indicative of the energy of a molecular vibration. Raman scattering is a very inefficient process, resulting in a low detection sensitivity that is incompatible with biological samples. In order to overcome weak signals, plasmonic nanostructures, such as Au and Ag, have been utilized in an approach termed SERS. Raman signal enhancement occurs when a molecule is located within the near field of the nanostructure’s LSPR (approximately the nanostructures diameter) and can result in up to 1014 enhancement compared to traditional Raman scattering (Nie and Emery 1997; Petryayeva and Krull 2011). Although SERS was first reported in 1973 and the cause of this effect has been heavily studied, the exact mechanism that results in surface enhancement has not been completely elucidated. There are two generally accepted mechanisms, the electromagnetic mechanism and the chemical mechanism (Caro et al. 2010). The electromagnetic mechanism requires the excitation of a nanostructure’s LSPR, which leads to an increase in the local EM
field surrounding the nanostructure and intensified electronic transitions of molecules located in close proximity to the nanostructure’s surface (Schatz et al. 2006). The chemical mechanism involves charge transfer interactions between the nanostructures and the molecules adsorbed onto the nanostructure’s surface (Otto and Futamata 2006). Of the two mechanisms, the electromagnetic mechanism is the dominant mode of enhancement. Like many of the bioanalytical approaches mentioned previously, the use of Au and Ag nanostructures allows for label-free SERS detection and molecular fingerprinting. Kneipp et al. (1998) reported the ability of Ag colloids to detect a single DNA base molecule (adenine), having intrinsic Raman scattering at 735 and 1,330 cm−1 due to the base’s ring-breathing mode. Label-free SERS has also allowed for cancer identification using cancertargeting AuNRs. In this work, El-Sayed and coworkers incubated anti-EGFR-AuNRs with cancerous and healthy cell lines and recorded the resulting SERS spectra (Huang et al. 2007). SERS spectra obtained from cancerous cells showed highly resolved molecular vibrations characteristic of bound AuNRs, while poorly resolved spectra were seen with healthy cells. More recently, label-free SERS detection has allowed for live cell molecular probing (Austin et al. 2013; Kang et al. 2012; Kneipp et al. 2002, 2006). Kneipp et al. (2002, 2006) were able to obtain SERS spectra of endosomal compartments in live epithelial and
macrophage single cells. Their use of unmodified AuNPs resulted in particle aggregation and aided in Raman enhancement. AuNPs have also been utilized to obtain SERS spectra of living HSC-3 cells throughout the entire life cycle (Kang et al. 2012). Since traditional methods for cell cycle analysis utilize DNA content to decipher between phases and the nucleus controls cellular function, AuNPs were functionalized with NLS peptides to promote AuNP nuclear localization. The AuNP confinement to a localized region allowed for low concentrations (0.05 nM) of AuNPs to be used and increased plasmon coupling between nanoparticles. The obtained SERS spectra indicated phasespecific SERS bands and resulted in a dynamic profile of cell cycle progression after release from G1 synchronization. Real-time SERS assessment of cancer cells treated with 100 μM cisplatin or 5-fluorouracil (5-FU) revealed three “SERS death bands” that were used to evaluate drug efficacy (Fig. 5a). The cell viability ratios from the SERS death bands produced were consistent with cytotoxicity measurements obtained from traditional absorbance-based assays (Austin et al. 2013). SERS Raman reporters, in conjunction with metal nanostructures, have also been heavily utilized in biological applications. Reporters are generally Raman active dyes with a distinct Raman vibrational band that can be detected in complex solution matrices. When reporters are adsorbed or covalently attached to a metal nanostructure,
Fig. 5 Surface-enhanced Raman scattering applications of AuNPs. a Live cell Rayleigh images and SERS spectra of cancer cells untreated (top) or treated with 100 M cisplatin (middle) or 5-FU (bot‑ tom). Apoptotic cell death and drug efficacy were determined by the increase or decrease in 500, 1,000, and 1,585 cm−1 band intensities. b In vivo SERS spectra obtained from tumor-targeted (top left) and nontargeted (top right) AuNPs. Raman reporter spectral signatures
were observed in tumors of nude mice (bottom left) treated with tumor-targeting (ScFv antibody-conjugated) AuNPs, while nontargeted AuNPs showed Raman signal at the liver. a Reprinted with permission from (Austin et al. 2013). Copyright. 2013 American Chemical Society. b Reprinted with permission from (Qian et al. 2008). Copyright. 2008 Nature Publishing Group
their Raman scattering results from the excitation of the nanostructure’s LSPR and does not require an excitation source in resonance. This allows for multiple targets to be identified at once. SERS multiplex detection was utilized in the simultaneous identification of different DNA and protein molecules as well as deciphering between co-cultured cancer cells (Hsin-Neng and Tuan 2009; Kang et al. 2010b; Lee et al. 2014; Maiti et al. 2011; Sun et al. 2007; Wang et al. 2013). Raman reporters have also been used to detect femtomolar concentrations of PSA. Grubisha et al. (2003) designed a 30 nm AuNP to contain Raman reporter, 5,5′-dithiobis(succinimidyl-2-nitrobenzoate) (DSNB), and anti-PSA antibodies. These functionalized AuNPs were incubated with increasing concentrations of f-PSA and provided a detection limit of 160 fg of f-PSA. Recently, silica-encased 90 nm gold cores functionalized with trans1,2-bis(4-pyridyl)ethylene (BPE) were able to be detected through bone using a combination of SERS and spatially offset Raman spectroscopy (SORS) (Sharma et al. 2013). Bone thicknesses (3–8 mm), probed in this work, mimicked those seen in the human skull and demonstrated the potential use of this technique to noninvasively probe the brain in vivo. Moreover, Raman reporters have enabled in vivo SERS imaging in other tissues (Keren et al. 2008; Maiti et al. 2012; Zavaleta et al. 2009). Nie and coworkers reported tumor detection in nude mice bearing a human head and neck squamous cell carcinoma (Tu686) xenograft tumor (Qian et al. 2008). AuNPs were functionalized with malachite green (Raman reporter), ScFv EGFR antibodies (targeting ligand), and PEG (particle stability) and were found to localize in the tumor site after tail vein injection. AuNPs that did not contain the targeting ligand showed Raman reporter signals in the liver (Fig. 5b). Jokerst et al. (2012) coupled SERS and photoacoustic imaging using AuNRs with an aspect ratio of 3.5 to detect and resect induced ovarian tumors in live mice. SERS imaging allowed for tumor and normal tissue margins to be clearly visualized. Metal‑enhanced fluorescence (MEF) Although fluorescent labels can suffer from low signal to noise ratios and photobleaching, they are commercially available and therefore are heavily used in biochemical assays. In an effort to circumvent these drawbacks, fluorescent labels are coupled with metal nanostructures in an approach termed metal-enhanced fluorescence (MEF). When a fluorophore is within 1–3 nm from the nanoparticle surface, its fluorescence is quenched due to electron transfer processes. However, if it is within 4–10 nm of the metal surface, its emission is significantly enhanced. The resulting fluorescent enhancement has been attributed to local EM field enhancement near the nanostructure’s surface as
well as a decrease in the fluorophore’s lifetime due to interaction with the nanostructure (Aslan et al. 2005). Immunoassays and nucleotide sensing are two MEF applications that have been heavily investigated. Geddes and coworkers reported successful RNA sensing via MEF using silver island films (SIF) (Aslan et al. 2006). Target RNA was tagged with TARMA, a fluorescent probe, and annealed to a DNA anchor probe in one step. The fluorescence emission of TARMA was significantly enhanced by the SIF, leading to a lower detection limit of 25 fmol and a signal to noise ratio greater than 20. This detection format, while less sensitive than traditional RNA assays, provides a more cost- and time-effective approach to RNA detection as RNA target amplification is not required. MEF has also been utilized to study supramolecular complexes, such as the ribosome (Bharill et al. 2010; Mandecki et al. 2008). Nanoparticle surface energy transfer (NSET) Many biological applications, especially those that probe protein interaction and enzyme activity, utilize Förster resonance energy transfer (FRET). FRET is a well-studied energy transfer mechanism between two fluorescent molecules that are separated by less than 10 nm. Due to their small separation, energy can be passed from one fluorophore (donor) to the other fluorophore (acceptor) through a nonradiative process (Jue 2010). This energy transfer results in an increase in the acceptor’s fluorescence emission and a decrease in the donor’s fluorescence. The small distance separations (